Yuh J.Chao
Mem.ASME
Department of Mechanical Engineering,
University of South Carolina,
Columbia,SC 29208
email:chao@sc.edu
Ultimate Strength and Failure
Mechanismof Resistance Spot
Weld Subjected to Tensile,Shear,
or Combined Tensile/Shear Loads
Strength tests were performed to reveal the failure mechanisms of spot weld in lapshear
and cross tension test samples.It is shown the while the lapshear (cross tension) sample
is subjected to shear (normal) load at the structural level the failure mechanism at the
spot weld is tensile (shear) mode at the materials level.Based on the observed failure
mechanism,stress distribution is assumed and related to the far ﬁeld load for the lap
shear and cross tension test samples.It appears that the failure load of the cross tension
sample is 74 percent of the lapshear sample based on the classical von Mises failure
theory.The theoretical model is further extended to the mixed normal/shear loading
condition.Data from strength tests as well as ﬁnite element numerical method are used to
validate the model.Finally,the utility of the model in accessing the failure strength of spot
welds is discussed.@DOI:10.1115/1.1555648#
1 Introduction
Spot weld made by resistance welding has been widely used in
joining sheet metal for auto body since 1950’s and is the primary
method of joining in ground vehicle industry.A modern vehicle
typically contains 2000 to 5000 spot welds.The strength of the
spot weld under quasistatic,impact,and fatigue loading condi
tions is therefore extremely important to the durability and safety
design of automobiles.In this paper,we focus our attention on
the failure behavior of spot weld under quasistatic overload
condition.
Although the spot weld has been used extensively,a simple
failure criterion that is able to predict the failure strength of a spot
weld subjected to various loading conditions does not exist.Con
ventional practice in industry is to perform extensive tests to ob
tain sufﬁcient data sets for design purpose @1,2#.The drawback of
this approach is that there are simply too many variables to con
sider,e.g.,welding parameters,sheet thickness,weld nugget size
for a given material.Consequently,it is costly to develop a mean
ingful and useful database.A veriﬁed,mechanics based failure
theory would be very useful to the designers and signiﬁcantly
reduce the number of test required and thus the cost involved.
Due to its complex geometry,analytical solution for stresses in
a spot weld is difﬁcult to obtain.Radaj @3#,Radaj and Zhang @4#,
and Zhang @5– 8#have adopted a fracture mechanics approach and
provided very detailed stress distribution around a weld nugget.
The derived linear elastic stress intensity factor solutions are
mathematical in nature and its practical application to the failure
of spot weld under monotonic loading has not been fully realized.
Wung @9#and Wung et al.@10#have recently reported the fail
ure strength of spot weld under inplane torsion and advocated the
force based failure criterion which is used in commercial ﬁnite
element code such as LSDYNA3D.
Zuniga and Sheppard @11#performed failure test of spot weld
on high strength steel and studied detailed failure mechanisms of
lapshear and coach peel samples.One of the main ﬁndings from
their work is that the failure mechanism for lapshear sample is
localized necking ~shear localization!in the base metal and near
the boundary between HAZ and base metal.Because of this ﬁnd
ing they then attempted using the plastic strain in the thickness
direction near the weld nugget as the failure criterion to interpret
the strength of spot weld.
Barkey et al.@12#and Lee et al.@13#designed a test sample and
a ﬁxture such that a spot weld test sample can be loaded under
pure shear,mixed shear/normal,or pure normal load by changing
the loading position of the ﬁxture.Ultimate strength data of spot
welds using the ﬁxture were reported and curve ﬁtted to a force
based failure criterion for design consideration.Similarly,Lin
et al.@14#reported another mixed mode test ﬁxture and some test
results.
At the University of South Carolina,weldability,failure mecha
nism and strength of spot weld under static,fatigue and impact
loading conditions are being investigated.Since interfacial mode
of failure in spot weld is generally not acceptable for automobile
applications due to its low load carrying and energy absorption
capability we ﬁrst studied the mechanics aspect of failure mode of
spot weld,i.e.,under what conditions a spot weld would fail in the
nonacceptable interfacial mode ~or the acceptable nugget pullout
mode!@15#.Having the interfacial mode of failure excluded,cur
rent paper as the second paper in the series addresses the ultimate
strength and failure mechanisms of spot weld subjected to tensile,
shear or combination of the two,under the assumption that the
weld fails in the pullout mode.The objective of this study is to
develop an engineering failure criterion for spot weld in thin sheet
metals under nugget pullout mode.Failure of spot weld under
impact loading as well as fatigue loading will be the subject of
future reports from our investigation.
To develop the failure criterion of spot welds,we ﬁrst per
formed the strength test using cross tension and lapshear ~or
tensileshear!samples made of a high strength steel.The cross
tension ~lapshear!sample geometry is chosen as a representative
case for predominantly opening ~shear!load or a normal ~shear!
force to the weld.Observation during the test reveals the fracture
initiation site and pattern.Fractographs from the fractured surface
are examined and the fracture mechanisms are then identiﬁed.
Based on the fracture mechanisma stress distribution is developed
and related to the failure load or ultimate strength of the spot weld
for the two sample geometries.A mechanics based failure crite
rion for the spot weld is then established using classical von Mises
or Tresca criterion.Having the failure criterion for each of the two
Contributed by the Materials Division for publication in the J
OURNAL OF
E
NGI

NEERING
M
ATERIALS AND
T
ECHNOLOGY
.Manuscript received by the Materials
Division February 5,2002;revision received August 12,2002.Associate Editor:G.
Newaz.
Journal of Engineering Materials and Technology APRIL 2003,Vol.125 Õ 125
Copyright © 2003 by ASME
sample geometries established,i.e.,tensile and shear,we ﬁnally
extend the failure criterion to combined tensile/shear loading
mode.Comparison with our test data as well as those from open
literature indicates that the prediction based on the developed
theory is very credible.In the section of discussion,potential ap
plications of the developed theory in design are discussed.
2 Material,Welding,Ultimate Strength Testing,and
Results
A high strength steel with sheet thicknesses 1.2 mm,1.5 mm
and 2.0 mm was selected for the test.The engineering as well as
the true stressstrain curve at quasistatic loading rate ~0.025
mm/s!is shown in Fig.1.The true stressstrain curve includes the
Bridgman’s correction for necking following the procedure out
lined in @16,17#.Relevant material properties are obtained from
the stressstrain curve as upper and lower yield strength of 359
MPa ~52 ksi!and 345 MPa ~50 ksi!,respectively,ultimate tensile
strength 434 MPa ~63 ksi!,reduction in area or ductility 61 per
cent,and the fracturing stress and strain as 676 MPa ~98 ksi!and
0.95,respectively.The stressstrain curve indicates that the mate
rial is ductile with a median strain hardening,i.e.,a strain
hardening exponent of 0.17.Its carbon content is less than 0.1
percent and magnesium less than 1 percent.The material is close
to HSLA ~high strength low alloy!Grade 50 steel or cold rolled
340 steel.
Cross tension samples composed of two 50.8 mm ~2 inches!
wide by 152.4 mm ~6 inches!long coupons and lapshear samples
from two 38.1 mm ~1.5 inches!by 152.4 mm ~6 inches!coupons
are spotwelded,as shown in Fig.2,with a square overlap area.
These sample dimensions follow the recommendation by SAE
@18#and have sufﬁcient widths to not affect the strength of the
weld @19#.
Welding was done using a 100 KVAspot welder machine using
ZTrode electrode cap that is Zirconium Copper based with a 7.87
mm radius hemispherical dome cap.The cap also has a ﬂat tip
face of 4.8 mm in diameter.Before welding,hand robbing using
cloth with acetone was applied to remove grease and dirt from the
coupon surface.
It is well known that both the interfacial failure and excessive
expulsion reduce the strength of a spot weld,partly due to the
small size of the nugget formed in welding and the porosity
present in the weld,respectively.The welding schedules,listed in
Table 1,are determined after several trials guided by industry
standards such as AWS @18#and strength tests using lapshear
sample geometry such that neither interfacial failure nor excessive
expulsion would occur.The resulted nominal ~average!weld nug
get diameters are 7.1 mm,7.26 mm,and 7.58 mm,respectively
for the 1.2 mm,1.5 mm,and 2.0 mm sheets.These weld nugget
sizes satisfy the conditions set by the predictive model @15#that
ensures pullout failure mode of the weld nugget.
Strength testing was performed on a MTS universal tensile test
ing machine with a rate 1.524 mm/min ~0.001 inch/sec!that is
nearly quasistatic.Test ﬁxtures for the cross tension samples
were fabricated according to AWS @18#.The displacement in the
lapshear sample was recorded using an extensometer with 50.8
mm ~2.0 inches!gage length.The stroke ~or machine!displace
ment was used for the cross tension sample.The load and dis
placement histories were simultaneously recorded during the test
ing.Tests were terminated as the two coupons of a test sample
separated completely.
Figure 3 shows schematically the loaddisplacement curves as
observed from the tests.It is seen that in the lapshear test the
loaddisplacement curve exhibits a nonlinear region before reach
ing the peak load.This part is very similar to the stressstrain
curve of ductile metals such as that shown in Fig.1 and is attrib
uted to the strain hardening of the material.The load starts to drop
as the crack initiates.As the crack propagates along the circum
ference of the nugget ~i.e.,pullout failure!the load drops gradu
ally.The shape of the ‘‘tail’’ of the curve depends upon the post
failure mode,i.e.,a long tail corresponds to a partial ~typically
onehalf!nugget pullout and subsequent tearing of base metal
along the loading direction and a short tail corresponds to com
plete nugget pullout.In the cross tension case,the displacement is
large relative to the lapshear sample and a nearly linear curve is
maintained until failure.The load drops to zero quickly immedi
ately after failure and the failure mode is typically clean and com
plete nugget pullout.
Batches AC in Fig.4 shows the test results in term of ultimate
strength ~or peak load!,which corresponds to the crack initiation
of the spot welds based on the observation during the tests.It is
seen that the ultimate strength of the spot weld is a function of ~a!
sample geometry—lapshear samples have higher strength than
the cross tension samples,~b!thickness of the sheet—thicker cou
pon has higher strength,and ~c!weld nugget size—weld with
larger nugget fails at a higher load.These trends are well known
and documented in industry.An unresolved and challenging issue
in this type of data is ‘‘can one develop a mechanics based model
such that this behavior can be predicted quantitatively?’’ In the
following sections we attempt to address this issue by studying the
failure mechanisms and then develop an analytical solution for
predicting the ultimate strength of spot weld.
3 Failure Mechanisms
LapShear Sample.Observation during tensile test of lap
shear samples reveals the failure process as schematically demon
strated in Fig.5.As the sample is pulled initially,the weld nugget
Fig.1 Engineering and true stressstrain curves for the HSLA
steel tested
Fig.2 Cross tension and lapshear test sample geometries
126 Õ Vol.125,APRIL 2003 Transactions of the ASME
experiences a rotation ~see Fig.5~b!!,which essentially aligns the
nugget with the loading line.In stage ~c!the material surrounding
the nugget is subjected to a predominantly tensile load and the
deformation near the nugget is similar to a rigid button embedded
in a ductile sheet.As the load increases,localized necking of the
sheet metal occurs at the two apices,i.e.,u50 deg and 180 deg at
locations near the juncture of the nugget and the base metal.Note
that these two points are on the two different pieces of the cou
pons.Fracture then initiates at one of these two points ~stage ~c!!
when the ductility of the sheet material is reached.Eventually
pullout failure of the weld occurs as the initial crack grows around
the circumference of the weld nugget.
Figure 6 is taken from the surface of a test sample.The loading
was stopped and reduced to zero as the fracture was ﬁrst observed
during the tensile test of this sample.The dark hairline at the
lower circumference of the nugget is the crack indicating the frac
ture initiation site.As can be seen from the ﬁgure,the fracture
initiation site is at the location u50 and some crack propagation
~2 to 4 mm!along the circumference of the weld nugget already
occurred on this sample.
Note that similar feature of those demonstrated in Fig.5 is ﬁrst
reported by Zuniga and Sheppard @11#and later by Lin et al.@14#.
Table 1 Welding schedule for the steel sheet
Thickness
of the
sheet
~mm!
Weld
Time
~cycles!
at 60 Hz
Hold
Time
~cycles!
at 60 Hz
Weld
Current
~kA!
Weld
Force
~N!
Nominal
Nugget
Diameter
~mm!
1
2
Nominal
Nugget
Thickness
~mm!
%
Nugget
Indentation
1.2 14 2 10 2,982 7.1 0.94 22
1.5 21 5 11 4,228 7.26 1.17 22
2 28 5 12 5,340 7.58 1.3 35
Fig.3 Schematics showing the loaddisplacement curves of
lapshear and cross tension samples
Fig.4 Ultimate strength of the spot welds;batch A,B,CUSC
data Batch D,Zuniga and Sheppard 11;batch E,Sawhill and
Furr 24 some data are shifted horizontally for clarity
Fig.5 Global deformation and failure process of a lapshear
spotweld sample:a initial conﬁguration,b nugget rotation
align ﬁrst with the loading line ;c stretching,thinning,and
necking,and d tensile fracture due to localized necking.
Fig.6 Fracture initiation site of a lapshear spotweld sample.
The hairline at the bottom of the nugget is the crack.
Journal of Engineering Materials and Technology APRIL 2003,Vol.125 Õ 127
Optical micrographs from a sequence of deformation pattern of
lapshear sample from @11#are reproduced here as Fig.7.Figure 7
clearly shows the stages of failure process development in a lap
shear sample—~a!,~b!,and ~c!showing the progress of the local
ized necking at a position near the weld nugget edge and ﬁnal
fracture in ~d!.
The observation and Figs.5–7 demonstrate that the failure
mechanism of lapshear sample at the material level is ‘‘tensile,’’
even though the global loading mode to the test sample is shear.
To further verify this point,a broken sample was cut,prepared and
the fracture surface at u50 deg was examined under a scanning
electronic microscope ~SEM!.Figure 8 shows a fractograph with
1,0003.The near circular dimples shown in Fig.8 indicate a
ductile and tensile fracture mechanism at the material level.
CrossTension Sample.The deformation pattern and failure
process of a cross tension sample is demonstrated in Fig.9.As the
sample is loaded,large bending deformation of the sheet occurs
initially ~Fig.9~b!!.Eventually the weld nugget is pulled out from
one coupon and stays with the other coupon ~Fig.9~c!!.To dem
onstrate this,a micrograph of the cross section of a failed 1.5 mm
specimen from Lin et al.@14#is reproduced here as Fig.10.Be
sides the initial global bending of the sheet,the failure can be well
characterized as through thickness shear around the weld nugget.
To further verify this failure mechanism,SEMexamination on the
fractured surface produces the picture shown in Fig.11.The elon
gated or ‘‘ﬁsh scale’’ dimples shown in Fig.11 indicate that the
fracture mechanism at the material level is ductile and shear,de
spite that the global loading mode to the sample is tensile.
Fig.7 Optical micrographs showing the stages of failure pro
cess of a lapshear sample:a,b,and c show the progress
of the localized necking and d ﬁnal fracture reproduced from
Zuniga and Sheppard 11
Fig.8 SEM fractograph 1000X of a lapshear sample:the cir
cular dimple rupture microstructure indicating tensile fracture
Fig.9 Global deformation pattern b and the weld nugget
pullout failure c of a cross tension sample
Fig.10 Optical micrograph of the cross section of a failed 1.5
mm specimen showing the pullout failure of the weld nugget
around the nugget circumference reproduced from Lin,et al.
14
Fig.11 SEM fractograph 1000X of a cross tension sample:
the ‘‘ﬁsh scale’’ rupture microstructure indicating shear
fracture
128 Õ Vol.125,APRIL 2003 Transactions of the ASME
4 Stress Analyses and Failure Load
Failure of spot weld is likely related to many parameters,e.g.,
residual stress,material inhomogeneity,welding parameters,
thickness,nugget size,and material properties of the HAZ and the
base metal.Attempts to include all these parameters in a failure
criterion would require substantial analytical,numerical,and ex
perimental efforts.Besides,any complex criterion would severely
limit its use in engineering applications.As such,we chose to
focus on developing an engineering approach by assuming a sim
pliﬁed stress distribution based on the identiﬁed failure mecha
nisms in lapshear and cross tension samples.These stresses can
then be related to the far ﬁeld applied load and subsequently fail
ure load or ultimate strength of the spot weld test sample.
For lapshear samples,since the failure is predominantly by
uniaxial tensile load and the weld nugget is circular,a harmonic
tensile stress distribution around the weld nugget,as shown in Fig.
12,is assumed.The distribution of the stress can be written as
s
~
u
!
5s
max
cos u (1)
where u5290 deg to 90 deg and s
max
is the maximum tensile
stress occurring at u50 deg.Due to symmetry there is another
similar stress distribution in u590 deg to 270 deg with s
max
at
u5180 deg acting on the other piece of the coupon.Equilibrium
condition requires that
P5
E
2p/2
p/2
s
~
u
!
d
2
tcos udu5
p
4
tds
max
50.785tds
max
(2)
where P is the applied tensile load at far ﬁeld.Equation ~2!relates
the local maximum stress to the far ﬁeld load.At the initiation of
fracture,Eq.~2!becomes
P
f
50.785tds
f
(3)
where t is the thickness of the base metal sheet or one half thick
ness of the weld nugget,d the diameter of the weld nugget,P
f
the
failure load or strength of the sample and s
f
the fracturing stress
of the material in tension.Here,‘‘failure’’ of the test sample is
deﬁned as the ‘‘fracture initiation’’ which corresponds to the peak
load as discussed earlier.
For cross tension test samples,since the failure is predomi
nantly by shear around the circular weld nugget,a harmonic shear
stress distribution around the weld nugget is assumed.As shown
in Fig.13,the shear stress distribution has four identical sectors to
reﬂect the symmetric condition of the loading.The distribution of
the stress in one sector can be written as
t
~
u
!
5t
max
cos 2u (4)
where t
max
is the maximum shear stress occurring at u50 deg,
180 deg ~and u590 deg,270 deg on the other piece of the cou
pon!.Equilibrium condition requires that
P52
E
2p/4
p/4
t
~
u
!
rtdu5tdt
max
(5)
where P is the applied tensile load in far ﬁeld.At the initiation of
fracture,Eq.~5!becomes
P
f
5tdt (6)
where t
f
is the fracturing stress of the material in shear.
Examining the failure loads of ~3!and ~6!,it appears that the
failure load is proportional to the thickness of the sheet metal and
the weld nugget diameter.Furthermore,two material properties,
fracturing stress in tension s
f
and fracturing stress in shear t
f
,are
present in Eqs.~3!and ~6!,respectively.These two can be related
to each other by using classical failure criteria.For example,for
ductile materials von Mises failure criterion requires t
f
50.577s
f
and Tresca requires t
f
50.5s
f
@16#.Using these failure
criteria and ~3!and ~6!,one has
P
f
cross tension
50.735 P
f
lapshear
von Mises
50.64 P
f
lapshear
Tresca (7)
Equation ~7!relates the failure load or the ultimate strength of a
spot weld tested in cross tension to lapshear sample geometry.
5 Effect of Weld Indentation
For steel,the thickness of the nugget of a spot weld is often less
than the thickness of the base metal sheet due to the applied pres
sure by the electrodes during the welding.The effect of this weld
indentation is more pronounced in thickgauged sheet than in thin
gauged sheet depending on the welding parameters.As shown in
Table 1,the percentage of reduction in thickness from the base
metal to the nugget is about 22 percent,22 percent,and 35 percent
corresponding to the thickness 1.2 mm,1.5 mm,and 2 mm,re
spectively.
For thin gauged sheet,i.e.,around 1 mm or less,the change in
thickness due to electrode indentation is typically not signiﬁcant.
As can be seen in Fig.7,the thickness of the nugget is nearly
twice of the base metal sheet thickness ~0.91 mm!,i.e.,no inden
tation,and the failure site is actually in the base metal.On the
other hand the fracture initiation site in a thicker sheet ~2 mm!,as
shown in Fig.6,is clearly at the corner where the change of
Fig.12 Assumed stress distribution around the weld nugget
in a lapshear sample
Fig.13 Assumed stress distribution around the weld nugget
in a cross tension sample
Journal of Engineering Materials and Technology APRIL 2003,Vol.125 Õ 129
thickness takes place.Stress concentration associated from the
geometry change at the location could also contribute to the ini
tiation of fracture.
Strictly speaking,in applying the formulas ~3!and ~6!,t is the
thickness where the necking or fracture occurs,i.e.,use t if frac
ture is in the base metal and t
n
~thickness of the nugget!if fracture
is along the circumference of the nugget.It was observed that the
fracture site depends on the welding schedule and thickness.How
ever,since in practice the nugget thickness t
n
is not measured and
reported,the base metal thickness t becomes the nature candidate
in all formulas in the current paper.Note that the recommended
practice by American Welding Society is the depth of depression
on sheet surfaces caused by welding electrodes not to exceed 25
percent of the sheet metal thickness @21#.The thickness of both
the base metal sheet and the weld nugget from our test is provided
in Table 1.The weld in the 2 mm thick sheet has excessive inden
tation apparently.It is anticipated that the error involved in using
the base metal thickness in Eqs.~3!and ~6!would not be signiﬁ
cant,relative to other factors,if the recommended practice in @21#
is followed.
6 Comparison With Numerical and Other Results
Zhang @5#performed detailed ﬁnite element analyses for spot
weld subjected to mixed far ﬁeld normal/shear load.As u50 in
@5#,the problem reduces to the lapshear sample and loading con
dition discussed in Section 4.The maximum tensile stress,calcu
lated numerically,which occurs at u50 shown in Fig.12,is re
ported in @5#for four cases that have different sample dimensions
and weld nugget diameters.Table 2 lists the results calculated
using Eq.~2!and the numerical solutions for the four cases from
@5#.The comparison indicates that Eq.~2!is indeed a very good
approximation.
Close examination of Eq.~2!,one can ﬁnd that this equation,
derived from the simple stress distribution shown in Fig.12,is
precisely the analytical solution developed from a more rigorous
analysis by Radaj and Zhang @22,23#.In @22,23#stress distribution
around a weld nugget is derived by assuming the weld nugget as
a circular rigid button embedded in an inﬁnitely large plate and
subjected to far ﬁeld tension.Since for steels,the yield stress in
the nugget is generally one to three times of the base metal,the
‘‘rigid button’’ assumption is indeed a good assumption for stress
analysis.This is also evidenced by the failure process discussed in
Section 3.
7 Comparison With Test Data fromCross Tension and
LapShear Samples
Assuming s
f
is a constant for a given material,using Eqs.~3!,
~6!,and ~7!one has
S
P
f
td
D
reference
5
P
f
td
for lapshear sample
5
S
0.785 P
f
0.577
D
51.36
P
f
td
for cross tension sample ~von Mises!
(8)
Equation ~8!can be used to convert the test data from one test
condition,i.e.,t,d,and P
f
,to a reference condition of a lapshear
sample,i.e.,another t,d,and P
f
of a lapshear sample.Test data
of batches AC shown in Fig.4 are normalized using ~8!with
respect to batch A,lapshear sample ~ALS!and plotted in Fig.14
with the same scale.As can be seen in Fig.14 the scatter of data
after normalization is greatly reduced compared to that shown in
Fig.4.It indicates that the developed model,i.e.,Eqs.~3!,~6!,and
~7!,is indeed respectable.In Fig.14,t
n
~half of the nugget thick
ness!is used for batches AC for a more precise comparison since
we have each nugget thickness measured individually.Batch C
data would be slightly lowered in Fig.14 if the sheet thickness t
were used because of its deeper indentation.However,it would
not affect the overall conclusion.
Zuniga and Sheppard @11#performed tests to study the failure
mechanisms of spot weld in lapshear and coach peel geometry.
They used a steel that is very close to ours and hence a direct
comparison is possible.Two groups of ultimate tensile strength,
82826147 N and 8536662 N,with a slightly different welding
schedules for the spot weld (t50.91 mm,d56.35 mm) are re
ported for the lapshear sample.These two are included in Fig.4
as batch D.The ultimate strength of batch D is considerably low
relative to batches AC because of its relatively thin gage and
small nugget size.However,when converting ~or normalizing!to
the reference weld nugget and sheet gage of batch ALS using Eq.
~8!,the ‘‘predicted’’ ultimate strength for the reference weld batch
ALS is inline with other test data as shown in Fig.14.
Sawhill and Furr @24#tested spot weld samples to study the
weldability of steel sheets.The materials tested include a wide
range of yield strength,i.e.,from plain carbon steel to HSLA and
the test sample geometries include cross tension,lapshear,coach
peel as well as inplane torsion.Envelope encompassing the weld
strength of coldrolled steels using lapshear and cross tension
samples is shown in Fig.15.The predicted failure load envelop
for cross tension samples,using the lapshear data in Fig.15 and
Eq.~7!,is also plotted in Fig.15 for comparison.As can be seen,
the prediction is very reasonable with Tresca being slightly better
than von Mises theory.
Fig.14 Failure loads normalized with respect to batch A,lap
shear sample ALS
Table 2 Maximum tensile stress NÕmm
2
predicted by Eq.2
and ﬁnite element analysis 5 P:load,d:nugget diameter,t:
sheet thickness,b:length,W:width
Eq.~2!FEA P ~N!d ~mm!t ~mm!b ~mm!W ~mm!
14.7 14.5 100 5.4 1.6 79.6 31
9.9 9.5 100 8.0 1.6 79.6 31
14.7 13.8 100 5.4 1.6 49.6 31
9.9 8.5 100 8.0 1.6 49.6 31
130 Õ Vol.125,APRIL 2003 Transactions of the ASME
8 Mixed NormalÕShear Loading
Having the stress distributions developed for spot weld sub
jected to normal force,i.e.,cross tension sample,and shear force,
i.e.,lapshear sample,an extension to mixed normal/shear loading
conditions is investigated in this section.The analytical result is
then compared with test data.
For spot weld loaded with a combination of normal and shear
forces,superposition of Eqs.~1!and ~4!can be used for the stress,
which leads to a biaxial stress ﬁeld.Using von Mises and Tresca
failure criteria for a biaxial stress ﬁeld,one has
1
3
@
2s
2
16t
#
1/2
5
&
3
s
f
von Mises
S
s
2
D
2
1t
2
5
S
s
f
2
D
2
Tresca (9)
Substituting Eqs.~1!and ~4!into ~9!and acknowledging that
points at u50,180 deg are the most critical points around the
weld nugget for failure,one obtains
1.623
S
P
S
td
D
2
13
S
P
N
td
D
2
5s
f
2
von Mises
1.623
S
P
S
td
D
2
14
S
P
N
td
D
2
5s
f
2
Tresca (10)
where P
S
5P cos ais the shear component and P
N
5P sinathe
normal component of the applied force P as shown in Fig.16.
Mixed mode test data from Lee et al.@13#is used here to vali
date the developed model.Mild steel with yield stress 170 MPa,
ultimate tensile strength 282 MPa and 0.89 mm thick sheet was
tested using two weld nugget sizes,4.3 mm and 6.4 mm.Failure
loads are reproduced in Fig.17.The average of the test data in the
pure shear case is used in ~3!to obtain the fracturing stress s
f
,
1562 MPa.Using this fracturing stress,the prediction of the fail
ure envelope or Eq.~10!is then plotted in Fig.17.As shown in
the ﬁgure,test data in the mixed mode region are somewhat lower
than the predicted.Nevertheless,considering the simplicity of the
proposed model,the comparison is reasonably good.
Note three different widths of test coupons are used in @13#,i.e.,
19 mm ~0.75 inch!,31 mm ~1.22 inch!,and 43 mm ~1.69 inch!.
Failure loads,shown in Fig.17,show an increasing trend with
increasing width.As studied by Zhou et al.@19#failure strength of
a spot weld is not affected by the width of a test sample when the
width is beyond a critical value.The strength decreases with the
width,as it is less than the critical value.For the sheet thickness
and nugget size used by Lee et al.@13#,the ﬁrst two widths are
apparently less than the critical width to ensure a ‘‘width indepen
dent’’ failure load.Our analytical model does not include the ef
fect of the width and this could contribute to the fact that better
comparison is obtained for wider samples shown in Fig.17.In
fact,if the prediction were made to each group of data with equal
width individually a better comparison would be obtained.
9 Discussion
The most intriguing result from the current work is that while
spot weld in a lapshear test sample is subjected to a global shear
load the failure mechanism of the weld at the microstructure level
is in fact tensile.On the other hand,while the spot weld in a cross
tension sample is subjected to normal load the failure mechanism
of the weld is shear.These failure mechanisms help us to develop
the applied loadstress relations,Eqs.~1–7!.And,accordingly the
failure load relations are able to explain why cross tension sample
always fails at a lower load than the lapshear sample containing
similar spot weld which is well known in industry but had lacked
mechanics based explanations.
As stated previously,the strength of spot welds can be related
to many factors such as residual stress,welding parameters and
material inhomogeneity.A rigorous mechanics based model,
which includes all these factors in predicting spot weld failure
would require signiﬁcant development and complex material con
stitutive models for the inhomogeneous materials in the weld,
thermalelectricalmechanical models for the welding and ad
vanced fracture criterion including the residual stress.Using the
Fig.15 Failure strength of lapshear and cross tension
samples made of cold rolled steels with various ultimate tensile
strength 24 and prediction by 7 The predicted is shifted to
the left Mises and right Tresca for clarity
Fig.16 TensileÕshear mixed mode test sample geometry 13
Fig.17 TensileÕshear mixed mode test data 13 and predic
tion by 10 Normalized loadÄfailure loadÕnugget diameter x
sheet thickness
Journal of Engineering Materials and Technology APRIL 2003,Vol.125 Õ 131
model in the current paper,however,detailed studies on the effect
of these factors to the failure load are circumvented.This conve
nience is achieved mainly by using a fracturing stress s
f
.Al
though the property s
f
is most likely dependent upon the welding
parameters and base metal material,in practice it can be obtained
easily from a simple lapshear tensile test and using Eq.~3!for a
batch of welds fabricated from a designated set of welding param
eters and sheet material.
Note that the ‘‘fracturing stress’’ for the HSLAmaterial studied
is 676 MPa from the uniaxial tensile tests shown in Fig.1.The
‘‘fracturing stress’’ as deﬁned in Eq.~3!is about 1780 MPa from
the spot weld test data shown in Figs.4 and 14.Theoretically,
some relationships between these two ‘‘material properties’’
should exist.Recall that in the early development of fracture me
chanics,i.e.,in the 1960’s,a critical stress criterion was often used
in predicting fracture event of solids.However,as of today,it is
still unclear why the critical stress determined from fracture tests
is much higher than the fracture stress fromuniaxial tensile test on
smooth specimens.Further studies along this direction to link the
basic material test data from smooth specimens to failure of
cracked solid or spot weld are deﬁnitely valuable.
An essential element in the current study,which distinguishes
itself from others,is to interpret the failure of spot weld at the
stress level.Using the tensile fracturing stress,the shear fracturing
stress and the classical failure theory we are able to link the failure
strength of spot weld from lap shear geometry to that from cross
tension geometry as well as the combined shear/normal loading
conditions.Practically,it implies that once the fracturing stress s
f
is determined from a simple lapshear test,ultimate strength of the
spot weld ~a!in cross tension sample,~b!with different nugget
size and base metal sheet thickness,and ~c!under mixed normal/
shear load,can be predicted using Eqs.~7!,~8!,and ~10!,respec
tively.This conclusion presents tremendous potential savings for
automotive industry that requires strength data of spot weld of
different sizes in different sheet gages in safety design.For ex
ample,using the test data shown in Fig.15,a steel with UTS
5434 MPa has the failure strength of 5,1356498 N if it is lap
shear and 31506850 N if it is cross tension sample.These failure
loads are based on sheet thickness t50.76 and weld nugget diam
eter d55.1 mm and are plotted in Fig.4 as batch E.The predicted
failure loads,after converting to t51.2 mm and d57.1 mm and
lap shear sample,i.e.,batch ALS,are then 11,32661094 N and
941762541 N.As shown in Fig.14,these predicted loads com
pare favorably to the test data of batches AD,although they are
about 10 percent to 15 percent lower than anticipated.It may be
concluded that the comprehensive test data provided in Fig.15 in
conjunction with Eq.~8!can be used by industry for preliminary
safety design of auto assemblies.
In the ﬁnite element ~FE!simulation of auto body under a crash
scenario,there are many unresolved issues.For examples,‘‘what
is the appropriate ~or least complex!FE model for the weld?’’ and
‘‘what is the failure criterion?’’ Using the equations developed in
this paper,a simple beam element may be used to simulate a weld
nugget connecting two sheets and failure of the weld can then be
quantiﬁed provided that the fracture stress s
f
is determined by
lapshear tests in advance.
This paper addresses the tension and shear in cross tension and
lapshear spot weld test sample geometries.Spot weld in auto
body assembly is generally subject to a combination of tension,
shear,torsion,as well as bending.To have a truly useful and
general engineering model for industry,further development for
spot weld under torsion and bending at the coupon level,e.g.,
coach peel sample,and validating the model through comparison
with test data from coupons and structural components,in quasi
static,fatigue and impact loading conditions are necessary.
Acknowledgment
Partial support of this work by NSF through grant
CMS0116238 and the encouragement from the Program Director,
Dr.Kenneth P.Chong are greatly appreciated.Nippert Company
generously supplied welding cap electrodes.Dr.Kenneth W.
Miller,formerly at USC,of St.Cloud State University,performed
the welding and some of the tests shown in Fig.4.Dr.X.Zhu
contributed to many discussions.Dr.P.C.Wang of General Motor
Corporation provided invaluable insight of spot welding from in
dustry point of view.
References
@1#Ewing,K.W.,Cheresh,M.,Thompson,R.,and Kukuchek,P.,1982,‘‘Static
and Impact Strengths of SpotWelded HSLA and Low Carbon Steel Joints,’’
SAE Paper 820281.
@2#VandenBossche,D.J.,1977,‘‘Ultimate Strength and Failure Mode of Spot
Welds in High Strength Steels,’’ SAE paper 770214.
@3#Radaj,D.,1989,‘‘Stress Singularity,Notch Stress and Structural Stress at
SpotWelded Joints,’’ Eng.Fract.Mech.,34~2!,pp.495–506.
@4#Radaj,D.,and Zhang,S.,1993,‘‘On the Relations Between Notch Stress and
Crack Stress Intensity in Plane Shear and Mixed Mode Loading,’’ Eng.Fract.
Mech.,44~5!,pp.691–704.
@5#Zhang,S.,2001,‘‘Approximate Stress Formulas for a Multiaxial Spot Weld
Specimen,’’ Weld.J.~Miami!,80~8!201s–203s.
@6#Zhang,S.,1999,‘‘Approximate Stress Intensity Factors and Notch Stresses for
Common SpotWelded Specimens,’’ Weld.J.~Miami!,78~5!,pp.1735–1795.
@7#Zhang,S.,1999,‘‘Stress Intensities Derived from Stresses Around a Spot
Weld,’’ Int.J.Fract.,99,pp.239–257.
@8#Zhang,S.,1997,‘‘Stress Intensities at Spot Welds,’’ Int.J.Fract.,88,pp.
167–185.
@9#Wung,P.,2001,‘‘A ForceBased Failure Criterion for Spot Weld Design,’’
Exp.Mech.,41~4!,pp.107–113.
@10#Wung,P.,Walsh,T.,Ourchane,A.,Stewart,W.,and Jie,M.,2001,‘‘Failure of
Spot Welds Under InPlane Static Loading,’’ Exp.Mech.,41~1!,pp.100–106.
@11#Zuniga,S.,and Sheppard,S.D.,1997,‘‘Resistance Spot Weld Failure Loads
and Modes in Overload Conditions,’’ Fatigue and Fracture Mechanics:27th
Volume,ASTM STP 1296,R.S.Piascik,J.C.Newman,and N.E.Dowling,
eds.,American Society for Testing and Materials,pp.469– 489.
@12#Barkey,M.E.,and Kang,H.,1999,‘‘Testing of Spot Welded Coupons in
Combined Tension and Shear,’’ Exp.Tech.,23~5!,pp.20–22.
@13#Lee,Y.,Wehner,T.,Lu,M.,Morrissett,T.,Pakalnins,E.,1998,‘‘Ultimate
Strength of Resistance Spot Welds Subjected to Combined Tension and
Shear,’’ J.Test.Eval.,26~3!,pp.213–219.
@14#Lin,S.H.,Pan,J.,Wu,S.,Tyan,T.,and Wung,P.,2002,‘‘Failure Loads of
Spot Welds under Combined Opening and Shear Static Loading Conditions,’’
Int.J.Solids Struct.,39,pp.19–39.
@15#Chao,Y.J.,2002,‘‘Failure of Spot Weld:A Competition Between Crack
Mechanics and Plastic Collapse,’’ Recent Advances in Experimental
Mechanics—In Honor of Isaac M.Daniel,Kluwer Academic Publishers,pp.
245–256.
@16#Dowling,N.E.,Mechanical Behavior of Materials,Prentice Hall,New Jersey.
@17#Zhang,Z.L.,Hauge,M.,Degard,J.,and Thaulow,C.,1999,‘‘Determining
Material True StressStrain Curve from Tensile Specimens With Rectangular
CrossSection,’’ Int.J.Solids Struct.,36,pp.3497–3516.
@18#ANSI/AWS/SAE/D8.997,1997,Recommended Practices for Test Methods
for Evaluating the Resistance Spot Welding Behavior of Automotive Sheet
Steel Materials,American Welding Society,Miami.
@19#Zhou,M.,Hu,S.J.,and Zhang,H.,1999,‘‘Critical Specimen Sizes for
TensileShear Testing of Steel Sheets,’’ Weld.J.~Miami!,78~9!,pp.305s–
312s.
@20#Materials and Applications,1998,Part II,Welding Handbook,4,8th edition,
American Welding Society.
@21#AWS D8.788,SAE J1188,1987,Recommended Practices for Automotive
Weld Quality—Resistance Spot Welding,American Welding Society.
@22#Radaj,D.,and Zhang,S.,1996,‘‘Anschauliche Grundlagen fur Krafte und
Spannungen in Punktgeschweisten Uberlappverbindungen,Konstruktion,’’ 48,
pp.65–71.
@23#Radaj,D.,and Zhang,S.,1996,‘‘Strukturspannungen am starren Kern in
endlich berandeter Platte,’’ Konstruktion,48,pp.195–199.
@24#Sawhill,J.M.,Jr.,and Furr,S.T.,‘‘Spot Weldability Tests for HighStrength
Steels,’’ SAE paper 810352.
132 Õ Vol.125,APRIL 2003 Transactions of the ASME
Enter the password to open this PDF file:
File name:

File size:

Title:

Author:

Subject:

Keywords:

Creation Date:

Modification Date:

Creator:

PDF Producer:

PDF Version:

Page Count:

Preparing document for printing…
0%
Comments 0
Log in to post a comment